Dear Label_Name,

Greetings! I hope you are well.

I am writing on behalf of an international publishing house, Science and Education Publishing, USA (http://www.sciepub.com).

Science and Education Publishing (SciEP) is a multidisciplinary open access publisher of Journals covering the fields of Science, Technology and Medicine. All SciEP publications are subject to high-quality peer review, editorial and production processes and are freely available online.

Welcome to the April, 2013 edition of SciEP newsletter, providing monthly summaries of articles on science & education related topics of interest to scientist and professionals. The mission of our journals is to provide an open access forum for publishing new findings on issues pertinent to scientific and academic field. We also invite you to submit original research papers, review articles, short reports, or case studies are considered for publication in our Multidisciplinary Journals.

American Journal of Public Health Research
DOI: 10.12691/ajphr-1-1-3

The Implementation of a Tele-Homecare System with Service Oriented Architecture and HL7 Message Transmission Standard
Ching-Sung Wang

American Journal of Medical and Biological Research
DOI: 10.12691/ajmbr-1-1-2

The Influence of Ethanol on Pyruvate Kinases Activity in Vivo, in Vitro, in Silico
Lelevich Sergey Vladimirovich, Khrustalev Vladislav Victorovich, Barkovsky Eugene Victorovich, Shedogubova Tatyana Aleksandrovna

American Journal of Medical Sciences and Medicine
DOI: 10.12691/ajmsm-1-1-1

Clinical and Histological Features in Wegener Granulomatosis
Li Cavoli Gioacchino, Passantino Rita, Bono Luisa, Tortorici Calogera, Ferrantelli Angelo, Giammarresi Carlo, Rotolo Ugo

American Journal of Infectious Diseases and Microbiology
DOI: 10.12691/ajidm-1-1-2

The Curse of Lymphatic Filariasis: Would the Continual Use of Diethylcarbamazine Eliminate this Scourge in Papua New Guinea?
Anne Lanham, Lillian Mwanri

We have released issues of some journals on February 2013.
American Journal of Public Health Research
American Journal of Medical Sciences and Medicine
American Journal of Medical and Biological Research
American Journal of Pharmacological Sciences
American Journal of Clinical Medicine Research
American Journal of Nursing Research
American Journal of Cancer Prevention
American Journal of Medicine Studies
American Journal of Infectious Diseases and Microbiology
American Journal of Cardiovascular Disease Research
American Journal of Biomedical Research
American Journal of Mechanical Engineering
American Journal of Microbiological Research
Journal of Preventive Medicine
American Journal of Food and Nutrition
American Journal of Hypertension Research
American Journal of Sports Science and Medicine
Journal of Cancer Research and Treatment
American Journal of Zoological Research
Journal of Biomedical Engineering and Technology
American Journal of Microbiological Research
Biomedical Science and Engineering

We are pleased to announce that submissions are now being accepted for peer review for all the journals across all our subject areas in SciEP.

Please submit your manuscript via our online submission system:
http://www.sciepub.com/author/signin

To unsubscribe from our mailing list, please click on the following link: unsubscribe

I am looking forward to hearing from you.

Kind regards,

David Rain
Email:join@sciepub.com
Science and Education Publishing (http://www.sciepub.com)

Influence of Growth Parameters on the Structural, Morphological and optical Properties of MgxZn1-xO Prepared by Metal Organic Chemical Vapor Deposition

K. Talla*, O. Sakho, P. D. Tall, C. B. Ndao, E. H. O. Gueye, M. B. Gaye, J. K. Dangbegnon, B. D. Ngom*, J. R. Botha, A. C. Beye

Groupe de physique du Solide et Sciences des Matériaux, Faculté des Sciences et Techniques Université Cheikh Anta Diop de Dakar (UCAD), B.P. 25114 Dakar-Fann Dakar (Sénégal)Groupe de physique du Solide et Sciences des Matériaux, Faculté des Sciences et Techniques Université Cheikh Anta Diop de Dakar (UCAD), B.P. 25114 Dakar-Fann Dakar (Sénégal)

Abstract: The influence of growth parameters on the structural, morphological and optical properties of MgxZn1-xO grown on sapphire substrate by metal organic chemical vapor deposition is studied. Pure oxygen gas is used as oxidant, bis-methyl-cyclopentadienyl magnesium ((MeCp)₂Mg) and diethyl zinc are used as Mg and Zn source, respectively. The growth temperature between and 320°C and 620°C, the VI/II (O/Mg, Zn) ratio ranging from 60 to 960 and the growth rate from 0.5 to 3.3 m/h, are systematically varied to determine their effects upon the above mentioned physical properties. Structural, morphological and optical properties of the thin films are characterized by means of X-Ray Diffraction (XRD), Scanning Electron Microscope (SEM) and Photoluminescence (PL). Experimental results indicate that the growth conditions are essential for engineering the growth of MgxZn1-xO. The optimum substrate temperature is found to be 420°C for the growth of MgxZn1-xO with a solid composition x below 30%, composition above which a phase segregation has been previously observed. With increasing temperature, strong parasitic reaction between (MeCp)₂Mg and oxygen is found to occur before they rich the substrate.

Keywords: MgZnO ternary alloys, MOCVD, bis-methyl-cyclopentadienyl magnesium ((MeCp)2Mg), Columnar growth

Citation: K. Talla, O. Sakho, P. D. Tall, C. B. Ndao, E. H. O. Gueye, M. B. Gaye, J. K. Dangbegnon, B. D. Ngom, J. R. Botha, A. C. Beye, Influence of Growth Parameters on the Structural, Morphological and optical Properties of MgxZn1-xO Prepared by Metal Organic Chemical Vapor Deposition. American Journal of Materials Science and Engineering, 4 (2). 20-25. January 2016. doi:10.12691/ajmse-4-2-1

1. Introduction

ZnO and its related alloys are currently extensively investigated for applications in optoelectronic and microelectronic device fabrication. MgxZn1-xO alloys are in particular needed for the fabrication of optoelectronic devices in the blue to the UV spectral regions. It is widely used in optical devices, such as light-emitting diodes, transparent conductive oxide, solar cells, laser, optical detector, photocatalysis and photoelectrochemistry [1]. In the process of the research, most of the growth of MgxZn1-xO films has been carried out using molecular beam epitaxy [2] and pulsed laser deposition [3]; few have been prepared using metal organic chemical vapour deposition (MOCVD) [4] in particular using pure oxygen gas as oxidant(see Ref. [5]). In most cases, tertiary butanol (TBOH) has been mainly used in the growth of ZnO and MgZnO. It has been proven difficult to obtain high quality MgxZn1-xO thin films in part because of the phase segregation, which appears at certain percentage of Mg content. Indeed, by alloying ZnO with MgO, the films retain the ZnO hexagonal structure for up to ~0.3 using TBOH in our reactor [5], such result is found by Ohtomo et al. [6] using oxygen gas. We have reported that the optical band gap can be tailored from 3.3 eV to 3.75 eV keeping the hexagonal structure [5]. Consequently, it causes a little lattice mismatch for the small difference between the ionic radius of Zn²⁺ (0.60 Å) and Mg²⁺ (0.57 Å) [7]. Alloying ZnO with Mg disturbs the structural properties, the density of structural defects, and causes alloy disorder effects. Therefore, due to the compositional unstable nature of the alloy, the presence of phase segregation and the presence of various defects causing numerous changes in the structural, morphological and optical properties, it appears essential to always investigate the effect of the MOCVD growth parameters. Such will improve and give insight on the material properties, and mostly on the various possible applications.

In this paper, the effect of growth parameters using oxygen pure gas as oxidant is investigated. Using the same MOCVD reactor (two inlet reactor tube), the effect of growth using TBOH as oxidant has been published (see Ref. [5]). The growth temperature and VI/II ratio is varied in order to examine, their effects on the structure, the morphology and optical properties. The effect of growth rate have been also studied. Suitable substrate would be chosen that favor growth orientation and optical properties of MgZnO itself to gain further improvement of crystal quality.

2. Experiments

MgxZn₁₋xO films were deposited on c-Al₂O₃ (0001) substrates using Ar as the carrier gas. (MeCp)₂Mg and DEZn were used as Mg and Zn sources, respectively. The total flow of the group II reactants, as well as the flow of the oxidizing agent (O₂), was fixed to yield a VI/II ratio of 60 (optimum for ZnO growth in our reactor). The Mg/Mg+Zn ratio was varied in order to change the Mg content in the vapour phase. MgxZn₁₋xO was deposited for 45 min (around 1–2 μm thickness) at 320, 420, 520 and 620°C. The VI/II also was varied from 60 to 960.

The Crystalline quality of the ZnO films was determined by X-ray diffraction using CuKα₁ radiation (λ=0.154 nm). Surface morphology of the samples was studied using a Jeol JSM-7001F field emission scanning electron microscope (FESEM). Mg content in the solid was determined by energy dispersive X-ray (EDX) analysis. For low temperature (4.2 K) measurements, the samples were immersed in liquid He. The samples were excited with the 325 nm line of a HeCd laser at a typical excitation power of 7 mW.

3. Results and Discussion

Figure 1 shows normalized PL spectra of MgxZn1-xO grown at different growth temperatures (320°C to 620°C) on c-Al₂O3 (0001), using pure oxygen gas as group VI source. The donor bound exciton (DoX) position varies slightly probably due to small compositional non-uniformity in Mg incorporation. As was the case for growth using TBOH [1], stacking fault-related transitions are observed at energies below that of the DoX line, labelled (e, Ao: free-to-bound). No obvious trend is observed in terms of Mg incorporation or strength of stacking faults-PL. The Mg content is higher at around 520°C, this is concluded repeating the experiment. It has been reported that the growth using (MeCp)₂Mg can be performed up to 800˚C using either O₂ or N₂O [5]. However with TBOH, degradation of the films occurs above 500°C, as well as a weakness in strength of the luminescence intensity. This is mostly due to the low reactivity, low cracking temperature of the alcohols and the heavy incorporation of carbon in the film. Although, the reported growth temperature using metal alkyls range between 200°C and 400°C, (MeCp)₂Mg seems useable up to higher temperatures, while still yielding good quality layers. The critical issue for growth at higher temperatures above 420°C, is the occurrence of a strong parasitic oxidation reaction between (MeCp)₂Mg/DEZn and the oxygen sources. This phenomenon occurs mostly at the inlet of the reactor tube and can cause an oxygen deficiency above the substrate. There is however a large disparity in published results with regards to higher temperature growth. This is most probably due to differences in the precursors used, but also due to the reactor setup (geometry and total pressure).

Figure 1. Low temperature (4.2 K) PL spectra of MgxZn1-xO films (xv=0.2) grown on c-Al₂O₃ at temperatures of 320 °C to 620 °C using O₂ as oxygen source

Figure 2 shows SEM images of the above mentioned thin films. The surface morphology changes significantly with substrate temperature. At ~320°C, uniform columnar crystals are obtained. This feature remains at 420°C, but the size of the columns increases. At 520°C, the surface exhibits faceted features with a variety of shapes. Some of these have the characteristic hexagonal symmetry. A further increase in temperature increases the size of the crystallites with no hexagonal columns observed. The growth temperature which seems to yield columnar growth is around 420°C. This temperature has also been found to be “optimum” for growth of ZnO using O₂. Energy Dispersive X-ray spectroscopy done on the sample grown at such optimized temperature allowed us to determine the Mg mole fraction of about 7%. In regard of this result, it can be concluded that the incorporation efficiency of the Mg within the use of (MeCp)₂Mg is extremely low.

Figure 2. SEM images of the MgxZn1-xO films grown on c-Al₂O₃ at various temperatures using O₂

Figure 3 shows the PL spectra (4.2 K) of MgxZn1-xO (xv=0.2) grown with different VI/II ratio on c-Al₂O₃ at 420°C. The spectra are dominated by the same DoX as for the sample above. In this case the stacking fault related transition is very small, this confirms the nonuniformity of the sample. No obvious change in Mg incorporation is detected. The VI/II ratio has no major effect in the Mg incorporation when using (MeCp) 2Mg. Increasing oxygen gas has no effect in the Mg incorporation efficiency.

Figure 3. Low temperature (4.2 K) PL spectra of MgxZn1-xO films (xv=0.2) grown on c-Al₂O3 with different VI/II ratios and using O₂ as oxygen source

Figure 4 shows SEM images of the same films. As for growth using TBOH, there is no significant change in the morphology of the film. The VI/II ratio does not affect the size or the shape of the column or crystals. In cross-sectional views (not shown), the columnar structures are observed grow normally to the substrate, which indicates, a preferred growth along the c-axis, as seen with XRD measurement. The availability (amount) of oxygen does not influence the initial nucleation stage at the interface. The temperature is the main driving force for the growth with oxygen pure gas.

Figure 4. SEM images of MgxZn1-xO films grown on c-Al₂O₃ with different VI/II ratios (60-960) using O2.

Figure 5 shows cross sectional SEM images of MgxZn1-xO grown on c-Al₂O₃ substrate at different growth rates 3.3 μm/h, 2.8 μm/h, 1.4 μm/h and 0.5 μm/h using oxygen as group VI source and xv=0.2. The growth temperature was 420°C. For all growth rates, the films reveal columnar growth with cone shape ends. The size of the columns varies depending of the growth rate. For low growth rate (0.5 μm/h), the film appears denser compare to high growth rate (3.3 μm/h). The variations in thicknesses are within experimental error. The deposition rate strongly influences the initial nucleation and coalescence of the films. It seems likely that a decrease in growth rate increases the coalescence of crystallite/grains formed during the initial deposition. The increase the group precursors strongly affect the film properties.

Figure 5. Cross sectional SEM images of MgxZn1-xO thin films grown on c-Al₂O3 substrate at different growth rates: 3.3 μm/h, 2.8 μm/h, 1.4 μm/h and 0.5 μm/h using oxygen as oxidant

Figure 6 shows the surfaces of the films. For growth rates of 3.3 μm/h and 2.8 μm/h, the surface features are similar to those of ZnO films. The films comprise dense columnar crystals with the films grown at 2.8 μm/h having the smallest columns. For growth rates of 1.4 μm/h and 0.5 μm/h, the surface features are comparable to those of MgxZn1-xO film with x≥0.2. The surfaces of the films drastically differ from these grown at higher growth rates and are considerably rougher. The lower growth rates seem enhance the formation of cubic structure (see inserts). Similar results have been observed by Kim et al. [8] when growing MgxZn1-xO.

Figure 6. SEM images of MgxZn1-xO grown on c-Al₂O₃ at different growth rate grown using oxygen at 420 °C and VI/II ratio=60

The lower growth rates possibly enhance the Mg deposition at the interface, causing the formation of an MgO rich layer/region, which has been observed by AES measurements on other films. The same effect was seen when growing higher Mg content films. Low growth rates seems to favor/force the cubic structure instead of the wurtzite structure, which is supported by XRD spectra in Figure 7, which shows the presence of MgO (111) peaks for film grown with lower growth rates. One can suggest therefore that lower growth rate accelerate the formation of phase segregation in the films.

Figure 7. XRD spectra of MgxZn1-xO grown on c-Al₂O₃ at growth rate of 1.4 μm/h and 0.5 μm/h using oxygen, a growth temperature of 420 °C and VI/II ratio of 60

Figure 8 shows low temperature (4.2 K) normalized PL spectra of the films. It seems reasonable to assume that the dominating peak in each spectrum is the stacking fault- related transition (e, A⁰). DoX transitions appear as shoulders on the high energy side of the stacking fault PL. The sample grown at a growth rate of 0.5 μm/h seems to have two DoX bands. For the sample grown at a rate of 1.4 μm/h, a shoulder at the lower energy side of the stacking fault PL is observed. This line is suggested to be another DoX transition. For all samples ZnO is present in a small amount as illustrated by the presence of NBE emission at ~3.36 eV. The sample grown with the lowest growth rate (0.5 μm/h) shows the lowest Mg incorporation. The presence of two DoX bands for the two lowest growth rates would indicate the existence of two bang gaps in the films. This would correlate with the deduction made from the morphologies in Figure 6.

Figure 8. Normalized low temperature PL spectra (4.2 K) of MgxZn1-xO grown on c-Al₂O3 at different growth rate (3.3 μm/h, 2.8 μm/h, 1.4 μm/h and 0.5 μm/h) with VI/II ratio of 60 and at substrate temperature of 420 °C

In MOCVD technique, the growth rate is proportional to the flux of atoms being transported, usually by diffusion, in the gas phase to the interface, which is identical to the flux of atoms crossing the interface into the solid [9]. The growth rate is mainly mass transport limited. Since the growth rate depends on the flow rate of species, then the source type of material will strongly influence the growth process. For example, Leys et al. [10] explained the cause of the lower incorporation efficiency of P in GaAsxP1-x to be dependent on growth rate, which influences the dwell time of As and P species on the surface. They attributed the lower incorporation efficiency of P to differences in the adsorption/desorption rate constants of the As and P species on the surface. InGaN, because of the higher desorption rate of In, the In incorporation efficiency is relatively low in the low growth rate region. As the growth rate increases the desorption rate of In is significantly reduced, due to the faster completion of the next layer, and consequently a higher In incorporation efficiency will be obtained [11]. Similar behaviour for Mg is suspected. From the results there is a trend in increased efficiency of Mg incorporation for higher DEZn flow rates. It is believed that during the growth of MgxZn1-xO the transport of (MeCp)₂Mg in the growth front depends strongly on the presence of DEZn. This observation is based on the fact that (MeCp)₂Mg and TBOH does not produce any MgO deposition on the substrate for the entire range of growth parameters studied. Due to the lower flow rate of DEZn at low growth rates Mg is significantly decreased at the growing site.

4. Conclusion

High VI/II ratios decrease Mg incorporation, possibly due to a stronger premature reaction between (MeCp)₂Mg and the oxidant, or a preferential heterogeneous interaction between the Mg and oxygen species on the growth front. Also, the stacking fault density is deduced to increase. The surface morphology is independent on the VI/II ratio. A Site blocking mechanism is suspected to result in reduced growth rates of MgxZn1-xO grown at high VI/II ratios (≥240). For VI/II ratios between 15 and 120, no major effect has been observed on the incorporation of magnesium.

For all growth rates, the films reveal columnar growth with cone shape ends. The size of the columns varies depending of the growth rate. For low growth rate (0.5 μm/h), the film appears denser compare to high growth rate (3.3 μm/h). The sample grown at a growth rate of 0.5 μm/h seems to have two DoX bands. Lower growth rate reveals existence of two bang gaps in the films. Mg incorporation is enhanced at higher growth rate.

Acknowledgements

This work is based upon research supported by the South African Research Chairs Initiative of the Department of Science and Technology and the SA National Research Foundation. The work is also supported through grants from the South African AMTS (AMTS07-29-E), the RSA/German BMBF agreement and by the NMMU. The authors would like to thank the Claude Leon Foundation Postdoctoral Fellowship for its support.

References

[1]   | Y. Hu, B. Cai, Z. Hu, Y. Liu, S. Zhang, H. Zeng, Current Applied Physics 15 (2015) 423-428.
[2]   | D. Jiang, J. Qina, X. Zhang, Z. Bai, D. Shen, Materials Science and Engineering B 176 (2011) 736-739.
[3]   | X. Wang, K. Saito, T. Tanaka, M. Nishio, Q. Guo, J. of Alloys and Compounds 627 (2015) 383-387.
[4]   | S. Han, Y.K. Shao, Y.M. Lu, P.J. Cao, F. Jia, Y.X. Zeng, W.J. Liu, D.L. Zhu, X.C. Ma, Journal of Alloys and Compounds 559 (2013) 209-213.
[5]   | K. Tala, J. K.Dangbegnon, M. C. Wagener, J. Weber, and J. R. Botha, J. Cryst. Growth, vol. 315, p. 297-300, 2011.
[6]   | A. Ohtomo, M. Kawasaki, T. Koida, K. Masubuchi, H. Koinuma, Y. Sakurai, Y. Yoshida, T. Yasuda, Y. Segawa, Appl. Phys. Lett. 72 (1998). 2466.
[7]   | N.B. Chen, C.H. Sui, Sci. Eng. B, Solid-State Mater. Adv. Technol. 126 (2006) 16.
[8]   | A. Lusson, N. Hanèche, C. Thiandoume, V. Sallet, and P. Galtier, J. Vac. Sci. Technol. B, vol. 23, pp. 1755-1759, 2009.
[9]   | B. K. S. K. M. a. H. K. C. D. C. Kim, Thin Solid Films, vol. 518, pp. 2975-2979, 2010.
[10]   | G. B. Stringfellow, Organometallic Vapor-Phase Epitaxy: Theory and Practice, San Diego: Academic Press, Inc., 1989.
[11]   | M. R. Leys, H. Titze, L. Samuelson, and J. Petruzzello, J. Cryst. Growth , vol. 93, p. 504, 1988.